Multiphase Characterization of Phase Equilibria in the Tb-Rich Corner of the Co-Cu-Tb System
- 13 Downloads
In recent years, the grain-boundary diffusion (GBD) and grain-boundary restructuring processes used in manufacturing Nd-Fe-B magnets show promise as procedures that allow one to increase their hysteretic characteristics. The processes are realized by adding various amounts of heavy-rare-earth metals (in the form of hydrides, oxides, intermetallic compounds, etc.) to powder mixtures. The additions decompose or melt during subsequent heat treatment, and their components diffuse into grains and remain within the grain-boundary phase and thus, increase the anisotropy field of the main-magnetic (Nd2Fe14B-based) phase and improve the grain-boundary structure, respectively. In the present study, we consider alloys near the Tb3(Co0.6Cu0.4) composition as such an addition, which is of importance in designing the microstructure of Nd-Fe-B permanent magnets allowing us to economically alloy them with terbium (via GBD) simultaneously making copper and cobalt parts of the magnet composition. The phase equilibria in the Tb-rich corner of the Co-Cu-Tb system near the Tb3(Co0.6Cu0.4) composition, which was found to be multiphase, are assessed based on electron microscopy studies, data from electron microprobe, x-ray diffraction, and differential thermal analyses, and from magnetic measurements. A portion of the isothermal section for compositions Tb-40 at.% Co-50 at.% Cu at 600°C was constructed. The copper solubility in Tb3(Co,Cu) and Tb12(Co,Cu)7, and Co solubility in the Tb(Cu,Co) compound were determined, which are up to 6.5, 14.5, and 10 at.%, respectively. The possibility of hydrogenation of the multiphase composition with the formation of TbHx, and fine Co and Cu powders, which are components for diffusion in manufacturing permanent magnets, is demonstrated.
KeywordsCo-Cu-Tb system copper solubility grain boundary diffusion Nd-Fe-B magnets partial isothermal section phase equilibria Tb-rich corner
We sincerely thank Dr. Bochvar N.R. for the useful discussion of the obtained results and Dr. A. Watson for his assistance in preparing the manuscript. This study was supported financially by the Ministry of Science and Higher Education of the Russian Federation, Agreement No. 14.616.21.0093 (Unique Identification Number RFMEFI61618X0093) and the Ministry of Education, Youth, and Sports of the Czech Republic, Project No. LTARF18031. Structural studies were performed using research infrastructure of the Centre of Collaborative Access for Functional Nanomaterials and High-Purity Substances, Baikov Institute of Metallurgy and Materials Science, Russian Academy of Sciences and of the Regional Materials Science and Technology Centre, VSB-TU, Ostrava (Czech Republic).
- 12.T.-H. Kim, S.-R. Lee, J.W. Kim, Y.D. Kim, H.-J. Kim, M.-W. Lee, and T.-S. Jang, Optimization of the Post-Sintering Annealing Condition for the High Cu Content Nd-Fe-B Sintered Magnet, J. Appl. Phys., 2014, 115, p 17A770-3Google Scholar
- 13.M. Ge Pan, H. Pengyue, Z. Zhu, J. Jiao, and Z. Zhao, Effects of Cobalt Addition on the Coercivity of Sintered NdFeB Magnets Prepared by HD Method, Zhongguo Xitu Xuebao, 2010, 28, p 247-251Google Scholar
- 20.G. S. Burkhanov, N. B. Kolchugina, Y. S. Koshkid`ko, J. Cwik, K. Skotnicova, T. Cegan, P. A. Prokof`ev, H. Drulis, A. Hackemer, Structure and Phase Composition of Tb3Co0.6Cu0.4 Alloys for Efficient Additions to Nd-Fe-B Sintered Magnets, METAL 2017 Confernce Proceedings, 24-26 May 2017, Tanger Ltd., Brno, Czech Republiuc, EU, p 1775-1781.Google Scholar
- 22.N. Kolchugina, T. Dobatkina, Co-Cu-Tb Ternary Phase Diagram Evaluation, In MSI Eureka, Effenberg, G. (Ed.), MSI, Materials Science International, Stuttgart (2017), Document ID: 10.36935.1.4.Google Scholar
- 23.T.B. Massalski, Binary Alloy Phase Diagrams, 2nd ed., The Materials Information Society, Materials Park, 1990, p 2Google Scholar
- 24.P.R. Subramanian, D.J. Chakrabarti, and D.E. Laughlin, , Phase Diagrams of Binary Copper Alloys, ASM International, Materials Park, 1990, p 1-3Google Scholar
- 26.A. Bezergheanu, R. Grasin, and R. Tetean, Magnetic Properties and Magnetocaloric Effect in Tb8Co16−xCux Compounds, Stud. Univ. Babes-Bolyai Phys., 2011, 56(2), p 39-46Google Scholar
- 29.O.I. Kharchenko, Ternary (Y,Ce)-Co-Cu Systems, Vestn. L’vovskogo Univ., Ser. Khimicheskaya, 1981, 23, p 58–61 (in Russian)Google Scholar
- 30.G.G. Devyatykh and G.S. Burkhanov, High-Purity Refractory and Rare-Earth Metals, International Science Publishing, Cambridge, 1997Google Scholar